*Materials Science Research India* Volume 02 No. (1) 39-44 (2004)

**NON-ISOTHERMAL KINETIC AND THERMODYNAMIC **

**STUDIES ON POLYESTERS AT DIFFERENT VISCOSITY **

**AVERAGE MOLECULAR MASSES **

**M.R.Tiwari*, LP. Pandey" and M.G.H.Zaidi' **

a

Department of Chemistry, Government Inter College, Pratappur Khatima (India)

b

DAV Post Graduate College, Dehradun Affiliated to H.N.B. University Garhwal (India)

c

Department of Chemistry, G.B. Pant University of Agriculture and Technology, Pantnagar, Udham Singh Nagar Uttranchal (India)

(Received, May 24, 2004)

**ABSTRACT **

Non-Isothermal kinetics of solid-state decomposition of Polybisphenol-A-Carbonate [PC; *(Mt\: *1.5 -
3.68 x 104_{) and polymethyl metacrylate [PMMA Miv1.55-3.52 x 10}4_{] has been investigated under nitrogen }
atmosphere in view to study the effect of molecular mass on their thermal decompositions in solid state.
Thermal data deduced through simultaneous thermogravimetric-differential thermal analysis-differential
thermo gravimetry [TG-DTA-DTG] was used for calculations of thermodynamic parameters through
Horowitz-Metzger and coats-Redfern methods, kinetics and mechanism of degradations of each polymer at
different molecular masses. [PC] showed two step decomposition with slower rate than [PMMA], which
showed single step decomposition at each of molecular mass ranges. It was observed that ester linkages in
[PC] backbone provided satisfactory over [PMMA] which contain ester linkages in side chain, to
Horowitz-Metzger, coats-Redfern methods kinetic equations of solid-sate decompositions In general,
Horowitz-Metzger methods have shown greater values of energy of activation than Coats-Redfern methods for
[PC]. Both of methods have provided a wide difference in frequency factor but almost same entropy change in
most of the cases* Thermodynamic and kinetic data were mostly satisfied for first order and zero order kinetics
in case of [PC] whereas were not satisfactory for [PMMA].

**Key words: Thermodynamic parameters, Horowitz-Metzger and Coats-Redfern methods. **

**INTRODUCTION **

The quality control and assessment in the industrial polymers have been found to be tedious and a series of experimental techniques were developed since past few decades1-2. Among such techniques, thermo analytical methods have emerged as a rapid and cost effective substitute over other analytical methods with reproducible results3-4. Most of the modern chemical and metalurgical industries employ process involving solid-state gas-solid interface reactions. A detailed knowledge of the thermodynamics, kinetic and reaction mechanisms of these thermally induced processes is of immense help to optimize and control the operating parameters leading to design of proper process equipment. Thermal analysis techniques like thermogravimetry (TG), differential thermal analysis (DTA), differential scanning calorimetry (DSC) etc, where the property of a substance measured, as a function of temperature is extremely useful in this context5. In addition, if

real time analysis of the product gases evolved during a thermally induced reaction will greatly enhance the possibility of correctily interpreting the kinetic data and arriving at most appropriate mechanism governing the process. Thus, knowledge of single particle kinetics becomes a pre-requisite for studying interface transport phenomena between moving gas stream and porous of solid materials6. Such single particle kinetics can be easily studied through simultaneous TG-DTA-DTG, evolved gas analysis EGA and thermo mechanical analysis TMA. Among such the technique of TG-DTA-DTG is frequently used as a. means of assessing the thermal stability and conveniently provide valuable information about kinetics and thermodynamics of the solid state decompositions of polymers and related heat resistant materials5-6

40 M.R. Tiwari **et al, Materials Sci. Res. India 02(1) 39-44 (2004) **

decomposition with hydrochloric acid. [PMMA] with viscosity average molecular mass (Mη): 1.55-3.52 x 104) was synthesized through benzoyl peroxide catalyzed free radial polymerization of freshly distilled monomer. The monomer and polymers were thermally characterized through simultaneous TG-DTA-DTG in nitrogen. Thermal data were used for calculations of thermodynamic parameters through Horowitz-Metzger7 and coats-Redfern methods8, kinetics and mechanism of degradations of each polymer at different molecular masses (Table 1)6.

**MATERIALS AND METHODS **

**Starting materials **

**(a)Poly bisphenol-A-Carbonate [PC]: **

[PC] was purchased with melt index 7 was purchased from Ms Sigma Aldrich Chemicals USA It was decomposed with aqueous HCI solution (10-30% v/v) at 100 ±1°C in the range of 0.5 to 1.0 h. This result a series of [PC] samples with different [PC] samples. Their molecular masses were deduced in tetrahydrofuran (K = 38.9 x 103 mL/g,α = 0.70) through Mark Houwink equation using Oswald's capillary viscometer9 and was found in the range of Mn=1.51-3.68 x 104.

**(b)Polymethyl metharcrylate [PMMA] **

PMMA solutions in benzene were prepared at a concentration of 10, 20 and 30% (VW). 50 ml of each solutions were separately polymerized in presence of benzoyl perioxide (0.1 M: 10 ml) for one hour at 100 ± 1 °C. PMMA of varying molecular masses were separatly isolated from each of the solutions, by evaporating the solvent. Viscosity average molecular masses of each of PMMA specimens was separated investigated in benzene (K = 5.5 x 10-3 mL, g , α = 0.76)9 and were found in the range of 1.55 - 3.52 x 104.

**(c)Thermal Analysis **

A simultaneous thermo gravimetric (TG) differential thermo-gravimetric (DTG) Differential thermal analysis (DTA) of each of the polymeric

samples has been performed over

NETZSCH-Geratebau GmbH Thermal Analyzer moder STA 409C.The sample size was ranged from 13 to 19.8 mg. The samples were allowed to decomposed in nitrogen at heating rate of 25°C/10.0 (K/min) 1400°C using alumina as a reference. All such thermo analytical procedures were executed at RSIC, Indian Institute of Technology (IIT), Madras.

Non-isothermal kinetics of solid-state decompositions of samples has been calculated from TG data to ascertain the rate controlling process according to the procedure reported by Sestak and Berggen and Satava6. In this procedure evaluations were made from different integral forms of kinetic expressions and the declaring rate equation based on diffusion was studied in terms of parabolic law satisfied to one dimensional transport (D1), two dimensional diffusion (D2), three dimensional diffusion according to Jander equation (D3) and three dimensional diffusion according to Ginstling-Brounshtein equation (D4) and the rate laws at one dimensional, zero order (R1), two

dimensional; cylindrical symmetry (R2) and three

dimensional spherical symmetry (R3) [Table I ].

**(d) Kinetics and Thermodynamics **

Thermogravimetric (TG) data of each of the polymers were evaluated for their weight loss (%) with reference to their temperature, decomposition stages involved and kinetic parameters with reference to their order (n) and energy of activation of thermal degradation (E), Entropy change (As) through a series of calculation procedures such as Horowitz-Metzger method6 and Coate-Redfern method7. Thermal properties [Table II] and thermodynamic data of the solid-state decompositions [Table III] of polymers are summerized.

**RESULTS AND DISCUSSION **

Thermal properties of [PC] and [PMMA] at different molecular masses were deduced through simultaneous TG-DTA-DTG in nitrogen. In all the cases [PC] showed two-step decompositions with a pair of sharp endotherms at DTA-TG-DTA. At all the molecular masses, both type of polymers showed increasing values for their respective crystallization, oxidation, maximum decomposition and melting temperatures with molecular masses. [PC] at molecular mass 1.51 x 104 indicating two sharp decomposition with glass transition Tg 239.0 and

M.R. Tiwari *et al, Materials Sci. Res. India 02(1) 39-44 (2004) * 41

**Table**-**1**:** Non-isothermal integral forms of kinetic expressions **
**for heterogeneous solid state reactions **

D1 α2

= Kt 1- dimensional diffusion (Parabolic law)

D2 (1-α)[-1n(1- α)] + α= kt 2- dimensional diffusion, cylinderal symmetry

D3 [1-(1- α)1/3_{] }

= Kt 3-dimensional diffusion, spherical symmetry (Jander equation)

D4 (1-2- α /3 -(1/ α) 2/3 = kt 3-dimensional diffusion, spherical symmetry (Giastiling Brownshtein equation)

F1 -1n (1- α) = kt Random nucleation; One nucleus on each particle (Mampel equation)

A2 [-1n>(1- α)] 1/2

= kt Random nucleation (Avrami equation I)

A3 [-1n(1- α)]1/3

= kt Random nucleation (Avrami equation II)

R2 1-(1- α) 1/2

= kt Phase boundary reaction; cylinderical symmetry

R3 l-(l- α) 1/3

= kt Phase boundary reaction; spherical symmetry

**TabIe**-**2:Thermal properties of polybisphenol-A carbonate and polymethyl **
**methycrylate [PMM A] at different molecular masses **

**Polymer ** **Mn2X10**
**4**

**TG [Weight residue (%) al **
**Temperature ("C)] **

**T**

**g** **Tc** **Tox** **Td** **Tm**

**20 ** **40 ** **60 ** **80 **

[PC] 1.51 632.0 466.6 455.5 433.3 239.0 388.8 570.9 695.0 524.8

2.65 661.1 472.2 461.1 433.3 403.9 452.9 581.5 705.3 531.4

3.68 666.6 483.3 466.6 450.0 503.3 535.9 573.9 654.5 654.5

[PMMA] 1.55 288.8 327.7 355.5 372.2 289.7 387.0 438.2 683.0 464.6

2.50 305.5 333.3 355.5 372.2 341.5 386.5 499.8 639.2 476.6

3.52 383.3 366.6 338.9 305.5 349.5 377.8 506.0 655.2 462.7

Tg Glass transition temperature empirically according to the relation Tg = 2/3 Tm 8

Tc Crystallization temperature Tox Oxidation temperature Td Decomposition temprature Tm Melting points

profiles at 471.1 °C and 588.4 °C at DTA with Tg at

529.3 °C. Thermal decomposition of [PMMA] was progressed at the higher rates than [PC] with lower thermal stability, (Table 2).

Kinetic and thermodynamic parameters of [PC] during thermal decomposition process were claculated for zero and first order kinetics in terms of energy of activation, frequency factors, and entropy changes according to Horwitz metzer (HM)7 and coats redfern (CR)8 methods. At molecular mass range 1.51 x 2.65 x 104 the values calculated for energy of activation were observed at lower values for CR method than HM which was calculated in the reversed order at molecular mass 3.68 x 104. At molecular mass 2.65x104 HM method showed negative values for entropy change than

other methods (Table 3).

42 M.R. Tiwari *et al, Materials Sci. Res. India 02(1) 39-44 (2004) *

**Table-3: Kinetic and thermodynamic parameters for [PC] **

**M**𝛈 ∆**T ** **DTA ** **Method ** **E ** **Z ** ∆**S **

1.51 x 104 755-1055K 723K

n = 1 CR 2.768 x 104

1.547 x105

1.486 x 105

HM 3.28 x105

1.447 2.795 x 105

n = 0 CR 4.153 x 104 1.647 x105 2.25 x105

HM 9.958 x 105

2.94 7.77 x 105

2.65x104 773-1123 K 734.1 K

n=1 CR 3.04 x105 1.086 x 105 1.51 x 105

HM 4.26 x 105 1.426 -36.029

n = 0 CR 4.965 x 104 1.111 x 105 2.49 x 105

HM 5.846 X 105 2.151 -47.559

3.68 x 104 773-1123K 734.1 K

n=1 CR 4.75 x 104 3.077 x 104 1.767 x 104

HM 1.51X106 3.80 -11.45

n=0 CR 7.134 x 104 4.134x104 2.865 x 104

HM 2.07 x 106

4.97 15.18

∆T = Temperature Range E = Energy Of Activation For Decomposition (Kg mol') Z = Frequency Factor (Min-1) ∆S = Entropy Change

1 2 3 4 5 6 7

**1/T(K) **

M.R. Tiwari *et*a/;*Materials Sci. Res. India 02(1) 39-44 (2004)* *43*

44 M.R. Tiwari *et*a/;*Materials Sci. Res. India 02(1) 39-44 (2004)*

Thermodynamics of decomposition process was studied by the solution of resective thermograms using Horowitz-Metzger (HM)7 and Coats-redfern methods equation.

Various patterns of Mechanism of [PC] with M𝛈= 1.51 x104

was studied by plotting the values of lig g (a) against T-1 (K) x 103 it has been observed that except D1 mechanism that is parabolic law for one dimentional transort all patterns were progressed almost according to same trends. These observations indicate that at higher temperature this compound indicated almost same behaviour towards various log g (α) functions. Among all such mechanism, the most linear plot were observed at A2 and A3 indicating

that mechanism of decomposition of this compound was satisfied according to Avrami-Erofeev Nuclei growth through either of two dimensional (A2) or three dimensional (A3) rate

determensional with spherical symmetry. [PC] sample with M𝛈 = 2.65 x104 indicated a

sudden increased in the value of log g(α) T = 3 x 10-3 K. Among all such variations the most linear plot of assign as Avrami-Erovee three-dimensional nuclear growth A3 [figure I].

Variation of log g(α) against T-1

(K) for [PC] sample with molecular mass 2.65 x104 indicated a sudden increase in log (α) at 3 x 10-3 K. For this case most linear plot was assigned to be according to Avrami-Erofeev nuclei growth A3. These

observations indicated that non-isothermal kinetics of solid state decomposition of [PC] almost satisfied Avrami-Erofeev nuclei growth mechanism with three dimensional growth [Figure II] and the extend to three dimensional (spherical symmetry) R3 for [PC] with molecular weight 3.68 x104 [Figure

III]. Due to the large rate of decompositions, mechanism of thermal of decomposition of [PMMA] samples has not been evalued according to these methods.

**REFERENCES **

1. Tanaka H, Koga N and Galway A K, *J Chem *
*Educ, ***72**(3), 251 (1995)

2. Brown M E, Dollimore D and Galway A K, In
*comprehensive chemical kinetics, *Vol.2 edited
by Bomford C H and Tipper C F H (Elsevier,
Amsterdam), 97 (1980)

3. Mackenzie R C, *Pure Apl Chem, 57, *1737
(1985)

4. Verma B P, Verma R K, Chandra M, Pandey S,
Mallick A K and Lata Verma, *Orient J Chem, *
6(3), 606 (1994)

5. Das S, Kamaruddin M, Krishnan R K and

Tyagi A K, *Ind J Chem Techol, ***5, **35-40 (1998)

6. Sestak J, Satava V and Wendlandt W W,
*Thermochem Acta, 7, *341 (1973)

7. Horowitz H H and Metzger G, *Anal Chem ***35, **
1464 (1963)

8. Coats A W and Redferm J D, *Nature *(London),
201, 68 (1964)